#------------------------------------------------------------------------------
#$Date: 2015-06-04 14:34:11 +0300 (Thu, 04 Jun 2015) $
#$Revision: 137956 $
#$URL: svn://www.crystallography.net/cod/cif/4/34/32/4343232.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4343232
loop_
_publ_author_name
'Read, Cory Michael'
'Smith, Mark D.'
'Withers, Ray'
'Zur Loye, Hans-Conrad'
_publ_section_title
;
 Flux Crystal Growth and Optical Properties of Two Uranium-Containing
 Silicates: A2USiO6 (A = Cs, Rb).
;
_journal_issue                   9
_journal_name_full               'Inorganic chemistry'
_journal_page_first              4520
_journal_page_last               4525
_journal_paper_doi               10.1021/acs.inorgchem.5b00364
_journal_volume                  54
_journal_year                    2015
_chemical_formula_moiety         'O6 Rb2 Si U'
_chemical_formula_sum            'O6 Rb2 Si U'
_chemical_formula_weight         533.06
_space_group_crystal_system      orthorhombic
_space_group_IT_number           71
_space_group_name_Hall           '-I 2 2'
_space_group_name_H-M_alt        'I m m m'
_symmetry_space_group_name_Hall  '-I 2 2'
_symmetry_space_group_name_H-M   'I m m m'
_audit_creation_method           SHELXL-2014/6
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.4916(6)
_cell_length_b                   12.6678(9)
_cell_length_c                   13.5077(9)
_cell_measurement_reflns_used    3457
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      30.534
_cell_measurement_theta_min      2.204
_cell_volume                     1453.02(17)
_computing_cell_refinement       'SAINT-Plus Version 6.45 (Bruker, 2001)'
_computing_data_collection       'SMART Version 5.631 (Bruker, 2001)'
_computing_data_reduction        'SAINT-Plus Version 6.45 (Bruker, 2001)'
_computing_molecular_graphics    various
_computing_publication_material  various
_computing_structure_refinement  'SHELXL-2014/6 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXS97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Bruker SMART APEX CCD diffractometer'
_diffrn_measurement_method       'omega and phi scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0437
_diffrn_reflns_av_unetI/netI     0.0203
_diffrn_reflns_laue_measured_fraction_full 1.000
_diffrn_reflns_laue_measured_fraction_max 1.000
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       18
_diffrn_reflns_limit_k_min       -18
_diffrn_reflns_limit_l_max       19
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_number            14697
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 1.000
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         30.554
_diffrn_reflns_theta_min         2.204
_diffrn_source                   'sealed tube'
_exptl_absorpt_coefficient_mu    35.790
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.5040
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS Version 2.05 (Bruker, 2001)'
_exptl_crystal_colour            orange
_exptl_crystal_density_diffrn    4.874
_exptl_crystal_description       'rectangular needle'
_exptl_crystal_F_000             1824
_exptl_crystal_size_max          0.080
_exptl_crystal_size_mid          0.070
_exptl_crystal_size_min          0.060
_refine_diff_density_max         2.271
_refine_diff_density_min         -2.993
_refine_diff_density_rms         0.369
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.088
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     61
_refine_ls_number_reflns         1282
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.088
_refine_ls_R_factor_all          0.0457
_refine_ls_R_factor_gt           0.0369
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0467P)²+29.7453P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0918
_refine_ls_wR_factor_ref         0.0965
_reflns_number_gt                1060
_reflns_number_total             1282
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            ic5b00364_si_002.cif
_cod_data_source_block           Rb2USiO6
_cod_database_code               4343232
_shelx_space_group_comment
; 
The symmetry employed for this shelxl refinement is uniquely defined 
by the following loop, which should always be used as a source of 
symmetry information in preference to the above space-group names. 
They are only intended as comments. 
;
_shelx_estimated_absorpt_t_min   0.162
_shelx_estimated_absorpt_t_max   0.223
_shelxl_version_number           2014/6
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z'
'-x, y, -z'
'x, -y, -z'
'x+1/2, y+1/2, z+1/2'
'-x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z+1/2'
'-x, -y, -z'
'x, y, -z'
'x, -y, z'
'-x, y, z'
'-x+1/2, -y+1/2, -z+1/2'
'x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, z+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
U1 U 0.2500 0.2500 0.2500 0.02121(14) Uani 1 2 d S . P
Rb1 Rb 0.0000 0.5000 0.15606(12) 0.0399(4) Uani 1 4 d S T P
Rb2 Rb 0.0000 0.0000 0.30222(12) 0.0311(3) Uani 1 4 d S T P
Rb3 Rb 0.0000 0.26261(13) 0.5000 0.0299(3) Uani 1 4 d S T P
Rb4 Rb 0.0000 0.19680(15) 0.0000 0.0352(4) Uani 1 4 d S T P
Si1 Si 0.1915(3) 0.5000 0.38785(17) 0.0142(5) Uani 1 2 d S T P
O1 O 0.2323(8) 0.3287(8) 0.1360(6) 0.064(3) Uani 1 1 d . . .
O2A O 0.2600(11) 0.3836(9) 0.3642(8) 0.026(2) Uiso 0.5 1 d . . P
O2B O 0.2505(12) 0.4153(9) 0.3149(9) 0.027(2) Uiso 0.5 1 d . . P
O3 O 0.0000 0.2427(8) 0.2670(8) 0.046(3) Uani 1 2 d S T P
O4 O 0.0000 0.5000 0.3840(8) 0.034(3) Uani 1 4 d S T P
O5A O 0.239(7) 0.529(4) 0.5000 0.019(4) Uiso 0.25 2 d S . P
O5B O 0.235(7) 0.459(4) 0.5000 0.019(4) Uiso 0.25 2 d S . P
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Rb Rb -0.9393 2.9676 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
U U -9.6767 9.6646 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 U1 O1 180.0 . 13
O1 U1 O3 91.8(4) . .
O1 U1 O3 88.2(4) 13 .
O1 U1 O3 88.2(4) . 13
O1 U1 O3 91.8(4) 13 13
O3 U1 O3 180.0 . 13
O1 U1 O2B 100.2(4) . 13
O1 U1 O2B 79.8(4) 13 13
O3 U1 O2B 90.0(3) . 13
O3 U1 O2B 90.0(3) 13 13
O1 U1 O2B 79.8(4) . .
O1 U1 O2B 100.2(4) 13 .
O3 U1 O2B 90.0(3) . .
O3 U1 O2B 90.0(3) 13 .
O2B U1 O2B 180.0 13 .
O1 U1 O2A 99.6(4) . .
O1 U1 O2A 80.4(4) 13 .
O3 U1 O2A 89.8(3) . .
O3 U1 O2A 90.2(3) 13 .
O2B U1 O2A 160.2(3) 13 .
O2B U1 O2A 19.8(3) . .
O1 U1 O2A 80.4(4) . 13
O1 U1 O2A 99.6(4) 13 13
O3 U1 O2A 90.2(3) . 13
O3 U1 O2A 89.8(3) 13 13
O2B U1 O2A 19.8(3) 13 13
O2B U1 O2A 160.2(3) . 13
O2A U1 O2A 180.0 . 13
O1 U1 Rb2 123.4(3) . .
O1 U1 Rb2 56.6(3) 13 .
O3 U1 Rb2 53.2(3) . .
O3 U1 Rb2 126.8(3) 13 .
O2B U1 Rb2 46.8(3) 13 .
O2B U1 Rb2 133.2(3) . .
O2A U1 Rb2 120.1(3) . .
O2A U1 Rb2 59.9(3) 13 .
O1 U1 Rb2 56.6(3) . 13
O1 U1 Rb2 123.4(3) 13 13
O3 U1 Rb2 126.8(3) . 13
O3 U1 Rb2 53.2(3) 13 13
O2B U1 Rb2 133.2(3) 13 13
O2B U1 Rb2 46.8(3) . 13
O2A U1 Rb2 59.9(3) . 13
O2A U1 Rb2 120.1(3) 13 13
Rb2 U1 Rb2 180.0 . 13
O1 U1 Rb3 50.0(3) . 13
O1 U1 Rb3 130.0(3) 13 13
O3 U1 Rb3 128.1(3) . 13
O3 U1 Rb3 51.9(3) 13 13
O2B U1 Rb3 68.8(3) 13 13
O2B U1 Rb3 111.2(3) . 13
O2A U1 Rb3 125.4(3) . 13
O2A U1 Rb3 54.6(3) 13 13
Rb2 U1 Rb3 114.36(3) . 13
Rb2 U1 Rb3 65.64(3) 13 13
O1 U1 Rb3 130.0(3) . .
O1 U1 Rb3 50.0(3) 13 .
O3 U1 Rb3 51.9(3) . .
O3 U1 Rb3 128.1(3) 13 .
O2B U1 Rb3 111.2(3) 13 .
O2B U1 Rb3 68.8(3) . .
O2A U1 Rb3 54.6(3) . .
O2A U1 Rb3 125.4(3) 13 .
Rb2 U1 Rb3 65.64(3) . .
Rb2 U1 Rb3 114.36(3) 13 .
Rb3 U1 Rb3 180.0 13 .
O1 Rb1 O1 169.5(3) 12 11_565
O1 Rb1 O1 94.9(3) 12 2_565
O1 Rb1 O1 84.1(3) 11_565 2_565
O1 Rb1 O1 84.1(3) 12 .
O1 Rb1 O1 94.9(3) 11_565 .
O1 Rb1 O1 169.5(3) 2_565 .
O1 Rb1 O4 95.27(16) 12 .
O1 Rb1 O4 95.27(16) 11_565 .
O1 Rb1 O4 95.27(16) 2_565 .
O1 Rb1 O4 95.27(16) . .
O1 Rb1 O2B 105.0(3) 12 .
O1 Rb1 O2B 82.2(3) 11_565 .
O1 Rb1 O2B 138.8(2) 2_565 .
O1 Rb1 O2B 51.0(3) . .
O4 Rb1 O2B 48.0(2) . .
O1 Rb1 O2B 138.8(2) 12 11_565
O1 Rb1 O2B 51.0(3) 11_565 11_565
O1 Rb1 O2B 105.0(3) 2_565 11_565
O1 Rb1 O2B 82.2(3) . 11_565
O4 Rb1 O2B 48.0(2) . 11_565
O2B Rb1 O2B 39.1(4) . 11_565
O1 Rb1 O2B 51.0(3) 12 12
O1 Rb1 O2B 138.8(2) 11_565 12
O1 Rb1 O2B 82.2(3) 2_565 12
O1 Rb1 O2B 105.0(3) . 12
O4 Rb1 O2B 48.0(2) . 12
O2B Rb1 O2B 83.1(4) . 12
O2B Rb1 O2B 96.0(4) 11_565 12
O1 Rb1 O2B 82.2(3) 12 2_565
O1 Rb1 O2B 105.0(3) 11_565 2_565
O1 Rb1 O2B 51.0(3) 2_565 2_565
O1 Rb1 O2B 138.8(2) . 2_565
O4 Rb1 O2B 48.0(2) . 2_565
O2B Rb1 O2B 96.0(4) . 2_565
O2B Rb1 O2B 83.1(4) 11_565 2_565
O2B Rb1 O2B 39.1(4) 12 2_565
O1 Rb1 Si1 76.87(17) 12 2_565
O1 Rb1 Si1 112.98(16) 11_565 2_565
O1 Rb1 Si1 76.87(17) 2_565 2_565
O1 Rb1 Si1 112.98(16) . 2_565
O4 Rb1 Si1 27.45(4) . 2_565
O2B Rb1 Si1 73.3(2) . 2_565
O2B Rb1 Si1 73.3(2) 11_565 2_565
O2B Rb1 Si1 25.9(2) 12 2_565
O2B Rb1 Si1 25.9(2) 2_565 2_565
O1 Rb1 Si1 112.98(16) 12 .
O1 Rb1 Si1 76.87(17) 11_565 .
O1 Rb1 Si1 112.98(16) 2_565 .
O1 Rb1 Si1 76.87(17) . .
O4 Rb1 Si1 27.45(4) . .
O2B Rb1 Si1 25.9(2) . .
O2B Rb1 Si1 25.9(2) 11_565 .
O2B Rb1 Si1 73.3(2) 12 .
O2B Rb1 Si1 73.3(2) 2_565 .
Si1 Rb1 Si1 54.90(8) 2_565 .
O1 Rb1 O3 135.06(18) 12 2_565
O1 Rb1 O3 50.87(18) 11_565 2_565
O1 Rb1 O3 50.87(18) 2_565 2_565
O1 Rb1 O3 135.06(18) . 2_565
O4 Rb1 O3 65.32(16) . 2_565
O2B Rb1 O3 91.4(2) . 2_565
O2B Rb1 O3 54.3(2) 11_565 2_565
O2B Rb1 O3 91.4(2) 12 2_565
O2B Rb1 O3 54.3(2) 2_565 2_565
Si1 Rb1 O3 68.25(14) 2_565 2_565
Si1 Rb1 O3 68.25(14) . 2_565
O2B Rb2 O2B 44.2(5) 14_445 8_455
O2B Rb2 O2B 112.7(5) 14_445 13
O2B Rb2 O2B 95.9(4) 8_455 13
O2B Rb2 O2B 95.9(4) 14_445 7_545
O2B Rb2 O2B 112.7(5) 8_455 7_545
O2B Rb2 O2B 44.2(5) 13 7_545
O2B Rb2 O3 106.7(3) 14_445 .
O2B Rb2 O3 62.8(2) 8_455 .
O2B Rb2 O3 62.8(2) 13 .
O2B Rb2 O3 106.7(3) 7_545 .
O2B Rb2 O3 62.8(2) 14_445 2
O2B Rb2 O3 106.7(3) 8_455 2
O2B Rb2 O3 106.7(3) 13 2
O2B Rb2 O3 62.8(2) 7_545 2
O3 Rb2 O3 162.4(4) . 2
O2B Rb2 O1 155.8(3) 14_445 13
O2B Rb2 O1 114.2(3) 8_455 13
O2B Rb2 O1 51.1(3) 13 13
O2B Rb2 O1 82.8(3) 7_545 13
O3 Rb2 O1 51.68(17) . 13
O3 Rb2 O1 134.32(16) 2 13
O2B Rb2 O1 51.1(3) 14_445 14_445
O2B Rb2 O1 82.8(3) 8_455 14_445
O2B Rb2 O1 155.8(3) 13 14_445
O2B Rb2 O1 114.2(3) 7_545 14_445
O3 Rb2 O1 134.32(16) . 14_445
O3 Rb2 O1 51.68(17) 2 14_445
O1 Rb2 O1 150.3(3) 13 14_445
O2B Rb2 O1 114.2(3) 14_445 7_545
O2B Rb2 O1 155.8(3) 8_455 7_545
O2B Rb2 O1 82.8(3) 13 7_545
O2B Rb2 O1 51.1(3) 7_545 7_545
O3 Rb2 O1 134.32(16) . 7_545
O3 Rb2 O1 51.68(17) 2 7_545
O1 Rb2 O1 83.7(3) 13 7_545
O1 Rb2 O1 88.7(3) 14_445 7_545
O2B Rb2 O1 82.8(3) 14_445 8_455
O2B Rb2 O1 51.1(3) 8_455 8_455
O2B Rb2 O1 114.2(3) 13 8_455
O2B Rb2 O1 155.8(3) 7_545 8_455
O3 Rb2 O1 51.68(17) . 8_455
O3 Rb2 O1 134.32(16) 2 8_455
O1 Rb2 O1 88.7(3) 13 8_455
O1 Rb2 O1 83.7(3) 14_445 8_455
O1 Rb2 O1 150.3(3) 7_545 8_455
O2B Rb2 O2A 10.8(3) 14_445 14_445
O2B Rb2 O2A 49.2(3) 8_455 14_445
O2B Rb2 O2A 104.1(3) 13 14_445
O2B Rb2 O2A 85.1(3) 7_545 14_445
O3 Rb2 O2A 109.3(2) . 14_445
O3 Rb2 O2A 57.7(2) 2 14_445
O1 Rb2 O2A 152.3(2) 13 14_445
O1 Rb2 O2A 57.1(2) 14_445 14_445
O1 Rb2 O2A 107.6(2) 7_545 14_445
O1 Rb2 O2A 92.3(2) 8_455 14_445
O2B Rb2 O2A 49.2(3) 14_445 8_455
O2B Rb2 O2A 10.8(3) 8_455 8_455
O2B Rb2 O2A 85.1(3) 13 8_455
O2B Rb2 O2A 104.1(3) 7_545 8_455
O3 Rb2 O2A 57.7(2) . 8_455
O3 Rb2 O2A 109.3(2) 2 8_455
O1 Rb2 O2A 107.6(2) 13 8_455
O1 Rb2 O2A 92.3(2) 14_445 8_455
O1 Rb2 O2A 152.3(2) 7_545 8_455
O1 Rb2 O2A 57.1(2) 8_455 8_455
O2A Rb2 O2A 51.8(4) 14_445 8_455
O1 Rb3 O1 136.8(4) 8_455 6
O1 Rb3 O1 71.5(3) 8_455 15_455
O1 Rb3 O1 92.6(3) 6 15_455
O1 Rb3 O1 92.6(3) 8_455 13
O1 Rb3 O1 71.5(3) 6 13
O1 Rb3 O1 136.8(4) 15_455 13
O1 Rb3 O3 123.58(17) 8_455 10_556
O1 Rb3 O3 52.26(15) 6 10_556
O1 Rb3 O3 52.26(15) 15_455 10_556
O1 Rb3 O3 123.58(17) 13 10_556
O1 Rb3 O3 52.26(15) 8_455 .
O1 Rb3 O3 123.58(17) 6 .
O1 Rb3 O3 123.58(17) 15_455 .
O1 Rb3 O3 52.26(15) 13 .
O3 Rb3 O3 170.8(4) 10_556 .
O1 Rb3 O5B 80.5(9) 8_455 3_556
O1 Rb3 O5B 137.7(6) 6 3_556
O1 Rb3 O5B 80.5(9) 15_455 3_556
O1 Rb3 O5B 137.7(6) 13 3_556
O3 Rb3 O5B 93.58(15) 10_556 3_556
O3 Rb3 O5B 93.58(15) . 3_556
O1 Rb3 O5B 137.7(6) 8_455 .
O1 Rb3 O5B 80.5(9) 6 .
O1 Rb3 O5B 137.7(6) 15_455 .
O1 Rb3 O5B 80.5(9) 13 .
O3 Rb3 O5B 93.58(16) 10_556 .
O3 Rb3 O5B 93.58(16) . .
O5B Rb3 O5B 77(2) 3_556 .
O1 Rb3 O2A 173.5(3) 8_455 10_556
O1 Rb3 O2A 49.7(3) 6 10_556
O1 Rb3 O2A 109.6(2) 15_455 10_556
O1 Rb3 O2A 90.7(2) 13 10_556
O3 Rb3 O2A 58.4(2) 10_556 10_556
O3 Rb3 O2A 126.8(2) . 10_556
O5B Rb3 O2A 93.3(9) 3_556 10_556
O5B Rb3 O2A 37.6(5) . 10_556
O1 Rb3 O2A 49.7(3) 8_455 12
O1 Rb3 O2A 173.5(3) 6 12
O1 Rb3 O2A 90.7(2) 15_455 12
O1 Rb3 O2A 109.6(2) 13 12
O3 Rb3 O2A 126.8(2) 10_556 12
O3 Rb3 O2A 58.4(2) . 12
O5B Rb3 O2A 37.6(5) 3_556 12
O5B Rb3 O2A 93.3(9) . 12
O2A Rb3 O2A 123.8(4) 10_556 12
O1 Rb3 O2A 90.7(2) 8_455 3_556
O1 Rb3 O2A 109.6(2) 6 3_556
O1 Rb3 O2A 49.7(3) 15_455 3_556
O1 Rb3 O2A 173.5(3) 13 3_556
O3 Rb3 O2A 58.4(2) 10_556 3_556
O3 Rb3 O2A 126.8(2) . 3_556
O5B Rb3 O2A 37.6(5) 3_556 3_556
O5B Rb3 O2A 93.3(9) . 3_556
O2A Rb3 O2A 85.5(4) 10_556 3_556
O2A Rb3 O2A 68.6(4) 12 3_556
O1 Rb3 O2A 109.6(2) 8_455 .
O1 Rb3 O2A 90.7(2) 6 .
O1 Rb3 O2A 173.5(3) 15_455 .
O1 Rb3 O2A 49.7(3) 13 .
O3 Rb3 O2A 126.8(2) 10_556 .
O3 Rb3 O2A 58.4(2) . .
O5B Rb3 O2A 93.3(9) 3_556 .
O5B Rb3 O2A 37.6(5) . .
O2A Rb3 O2A 68.6(4) 10_556 .
O2A Rb3 O2A 85.5(4) 12 .
O2A Rb3 O2A 123.8(4) 3_556 .
O2A Rb4 O2A 139.3(5) 15_454 13
O2A Rb4 O2A 77.7(4) 15_454 8_455
O2A Rb4 O2A 88.4(4) 13 8_455
O2A Rb4 O2A 88.4(4) 15_454 6_554
O2A Rb4 O2A 77.7(4) 13 6_554
O2A Rb4 O2A 139.3(5) 8_455 6_554
O2A Rb4 O5B 41.1(4) 15_454 15_454
O2A Rb4 O5B 107.1(8) 13 15_454
O2A Rb4 O5B 41.1(4) 8_455 15_454
O2A Rb4 O5B 107.1(8) 6_554 15_454
O2A Rb4 O5B 107.1(8) 15_454 13
O2A Rb4 O5B 41.1(4) 13 13
O2A Rb4 O5B 107.1(8) 8_455 13
O2A Rb4 O5B 41.1(4) 6_554 13
O5B Rb4 O5B 97(2) 15_454 13
O2A Rb4 O5A 41.9(4) 15_454 5_444
O2A Rb4 O5A 105.2(8) 13 5_444
O2A Rb4 O5A 41.9(4) 8_455 5_444
O2A Rb4 O5A 105.2(8) 6_554 5_444
O5B Rb4 O5A 2.6(19) 15_454 5_444
O5B Rb4 O5A 94.9(5) 13 5_444
O2A Rb4 O5A 105.2(8) 15_454 7_545
O2A Rb4 O5A 41.9(4) 13 7_545
O2A Rb4 O5A 105.2(8) 8_455 7_545
O2A Rb4 O5A 41.9(4) 6_554 7_545
O5B Rb4 O5A 94.9(5) 15_454 7_545
O5B Rb4 O5A 2.6(19) 13 7_545
O5A Rb4 O5A 92.3(19) 5_444 7_545
O2A Rb4 O1 52.2(3) 15_454 3
O2A Rb4 O1 168.5(3) 13 3
O2A Rb4 O1 96.5(3) 8_455 3
O2A Rb4 O1 104.7(3) 6_554 3
O5B Rb4 O1 83.1(8) 15_454 3
O5B Rb4 O1 144.59(14) 13 3
O5A Rb4 O1 85.2(8) 5_444 3
O5A Rb4 O1 144.44(17) 7_545 3
O2A Rb4 O1 104.7(3) 15_454 10
O2A Rb4 O1 96.5(3) 13 10
O2A Rb4 O1 168.5(3) 8_455 10
O2A Rb4 O1 52.2(3) 6_554 10
O5B Rb4 O1 144.59(14) 15_454 10
O5B Rb4 O1 83.1(8) 13 10
O5A Rb4 O1 144.44(17) 5_444 10
O5A Rb4 O1 85.2(8) 7_545 10
O1 Rb4 O1 76.9(3) 3 10
O2A Rb4 O1 96.5(3) 15_454 12
O2A Rb4 O1 104.7(3) 13 12
O2A Rb4 O1 52.2(3) 8_455 12
O2A Rb4 O1 168.5(3) 6_554 12
O5B Rb4 O1 83.1(8) 15_454 12
O5B Rb4 O1 144.59(14) 13 12
O5A Rb4 O1 85.2(8) 5_444 12
O5A Rb4 O1 144.44(17) 7_545 12
O1 Rb4 O1 70.8(3) 3 12
O1 Rb4 O1 116.4(3) 10 12
O2A Rb4 O1 168.5(3) 15_454 .
O2A Rb4 O1 52.2(3) 13 .
O2A Rb4 O1 104.7(3) 8_455 .
O2A Rb4 O1 96.5(3) 6_554 .
O5B Rb4 O1 144.59(14) 15_454 .
O5B Rb4 O1 83.1(8) 13 .
O5A Rb4 O1 144.44(17) 5_444 .
O5A Rb4 O1 85.2(8) 7_545 .
O1 Rb4 O1 116.4(3) 3 .
O1 Rb4 O1 70.8(3) 10 .
O1 Rb4 O1 76.9(3) 12 .
O2B Si1 O2B 88.3(9) . 11_565
O2B Si1 O5A 132.8(19) . .
O2B Si1 O5A 111.3(18) 11_565 .
O2B Si1 O5A 111.3(18) . 11_565
O2B Si1 O5A 132.8(19) 11_565 11_565
O5A Si1 O5A 26(3) . 11_565
O2B Si1 O2A 113.1(6) . 11_565
O2B Si1 O2A 28.6(5) 11_565 11_565
O5A Si1 O2A 83.6(18) . 11_565
O5A Si1 O2A 107.6(18) 11_565 11_565
O2B Si1 O2A 28.6(5) . .
O2B Si1 O2A 113.1(6) 11_565 .
O5A Si1 O2A 107.6(18) . .
O5A Si1 O2A 83.6(18) 11_565 .
O2A Si1 O2A 131.6(8) 11_565 .
O2B Si1 O4 107.7(5) . .
O2B Si1 O4 107.7(5) 11_565 .
O5A Si1 O4 106(2) . .
O5A Si1 O4 106(2) 11_565 .
O2A Si1 O4 110.7(4) 11_565 .
O2A Si1 O4 110.7(4) . .
O2B Si1 O5B 107.3(19) . .
O2B Si1 O5B 137(2) 11_565 .
O5A Si1 O5B 31.5(9) . .
O5A Si1 O5B 5(3) 11_565 .
O2A Si1 O5B 112.9(19) 11_565 .
O2A Si1 O5B 79.2(19) . .
O4 Si1 O5B 105(2) . .
O2B Si1 O5B 137.5(19) . 11_565
O2B Si1 O5B 107.3(19) 11_565 11_565
O5A Si1 O5B 5(3) . 11_565
O5A Si1 O5B 31.5(9) 11_565 11_565
O2A Si1 O5B 79.2(19) 11_565 11_565
O2A Si1 O5B 112.9(19) . 11_565
O4 Si1 O5B 105(2) . 11_565
O5B Si1 O5B 37(4) . 11_565
O2B Si1 Rb1 65.3(4) . .
O2B Si1 Rb1 65.3(4) 11_565 .
O5A Si1 Rb1 161.9(18) . .
O5A Si1 Rb1 161.9(18) 11_565 .
O2A Si1 Rb1 89.5(4) 11_565 .
O2A Si1 Rb1 89.5(4) . .
O4 Si1 Rb1 60.7(4) . .
O5B Si1 Rb1 157.2(19) . .
O5B Si1 Rb1 157.2(19) 11_565 .
O2B Si1 Rb2 47.1(4) . 13
O2B Si1 Rb2 47.1(4) 11_565 13
O5A Si1 Rb2 118.7(19) . 13
O5A Si1 Rb2 118.7(19) 11_565 13
O2A Si1 Rb2 66.8(4) 11_565 13
O2A Si1 Rb2 66.8(4) . 13
O4 Si1 Rb2 133.7(4) . 13
O5B Si1 Rb2 119(2) . 13
O5B Si1 Rb2 119(2) 11_565 13
Rb1 Si1 Rb2 73.02(5) . 13
O2B Si1 Rb3 80.8(4) . .
O2B Si1 Rb3 163.9(4) 11_565 .
O5A Si1 Rb3 84.8(17) . .
O5A Si1 Rb3 62.9(18) 11_565 .
O2A Si1 Rb3 165.9(4) 11_565 .
O2A Si1 Rb3 60.2(4) . .
O4 Si1 Rb3 65.06(18) . .
O5B Si1 Rb3 58.0(19) . .
O5B Si1 Rb3 88.8(19) 11_565 .
Rb1 Si1 Rb3 99.15(4) . .
Rb2 Si1 Rb3 126.45(3) 13 .
U1 O1 Rb1 112.2(4) . .
U1 O1 Rb3 103.3(3) . 13
Rb1 O1 Rb3 144.0(3) . 13
U1 O1 Rb4 104.5(4) . .
Rb1 O1 Rb4 91.43(18) . .
Rb3 O1 Rb4 85.2(3) 13 .
U1 O1 Rb2 95.2(3) . 13
Rb1 O1 Rb2 87.3(3) . 13
Rb3 O1 Rb2 83.68(16) 13 13
Rb4 O1 Rb2 159.2(3) . 13
O2B O2A Si1 70.3(12) . .
O2B O2A U1 78.6(12) . .
Si1 O2A U1 142.5(6) . .
O2B O2A Rb4 141.7(12) . 13
Si1 O2A Rb4 116.4(5) . 13
U1 O2A Rb4 101.0(4) . 13
O2B O2A Rb3 130.7(12) . .
Si1 O2A Rb3 94.3(4) . .
U1 O2A Rb3 90.4(3) . .
Rb4 O2A Rb3 87.5(3) 13 .
O2B O2A Rb2 43.1(10) . 13
Si1 O2A Rb2 87.1(5) . 13
U1 O2A Rb2 84.1(3) . 13
Rb4 O2A Rb2 98.6(3) 13 13
Rb3 O2A Rb2 172.5(4) . 13
O2A O2B Si1 81.1(12) . .
O2A O2B U1 81.6(12) . .
Si1 O2B U1 152.7(7) . .
O2A O2B Rb2 126.1(12) . 13
Si1 O2B Rb2 109.5(5) . 13
U1 O2B Rb2 97.7(4) . 13
O2A O2B Rb1 144.1(12) . .
Si1 O2B Rb1 88.8(5) . .
U1 O2B Rb1 92.8(4) . .
Rb2 O2B Rb1 89.8(3) 13 .
O2A O2B Rb4 30.5(10) . 13
Si1 O2B Rb4 91.2(5) . 13
U1 O2B Rb4 84.5(3) . 13
Rb2 O2B Rb4 95.6(3) 13 13
Rb1 O2B Rb4 174.3(4) . 13
U1 O3 U1 166.7(6) 8_455 .
U1 O3 Rb2 93.4(3) 8_455 .
U1 O3 Rb2 93.4(3) . .
U1 O3 Rb3 95.9(3) 8_455 .
U1 O3 Rb3 95.9(3) . .
Rb2 O3 Rb3 85.8(3) . .
U1 O3 Rb1 85.2(3) 8_455 .
U1 O3 Rb1 85.2(3) . .
Rb2 O3 Rb1 164.1(3) . .
Rb3 O3 Rb1 110.1(2) . .
Si1 O4 Si1 176.3(8) . 2_565
Si1 O4 Rb1 91.8(4) . .
Si1 O4 Rb1 91.8(4) 2_565 .
Si1 O4 Rb3 89.15(18) . .
Si1 O4 Rb3 89.15(18) 2_565 .
Rb1 O4 Rb3 117.52(16) . .
Si1 O4 Rb3 89.15(18) . 9_566
Si1 O4 Rb3 89.15(18) 2_565 9_566
Rb1 O4 Rb3 117.52(16) . 9_566
Rb3 O4 Rb3 125.0(3) . 9_566
O5B O5A O5A 168(10) 11_565 11_565
O5B O5A O5B 166(10) 11_565 .
O5A O5A O5B 2(7) 11_565 .
O5B O5A Si1 100(10) 11_565 .
O5A O5A Si1 76.9(17) 11_565 .
O5B O5A Si1 76(3) . .
O5B O5A Si1 100(10) 11_565 10_556
O5A O5A Si1 76.9(17) 11_565 10_556
O5B O5A Si1 76(3) . 10_556
Si1 O5A Si1 141(4) . 10_556
O5B O5A Rb4 58(10) 11_565 5
O5A O5A Rb4 133.8(9) 11_565 5
O5B O5A Rb4 136(8) . 5
Si1 O5A Rb4 109.7(18) . 5
Si1 O5A Rb4 109.7(18) 10_556 5
O5B O5A Rb3 25(10) 11_565 9_566
O5A O5A Rb3 142.5(9) 11_565 9_566
O5B O5A Rb3 140(8) . 9_566
Si1 O5A Rb3 91.6(19) . 9_566
Si1 O5A Rb3 91.6(19) 10_556 9_566
Rb4 O5A Rb3 83.7(12) 5 9_566
O5B O5A Rb4 155(10) 11_565 13
O5A O5A Rb4 37.8(9) 11_565 13
O5B O5A Rb4 40(7) . 13
Si1 O5A Rb4 88.5(18) . 13
Si1 O5A Rb4 88.5(18) 10_556 13
Rb4 O5A Rb4 96.0(14) 5 13
Rb3 O5A Rb4 179.7(18) 9_566 13
O5A O5B O5A 10(10) 11_565 .
O5A O5B O5B 12(10) 11_565 11_565
O5A O5B O5B 2(7) . 11_565
O5A O5B Si1 75(10) 11_565 .
O5A O5B Si1 72(3) . .
O5B O5B Si1 71.6(18) 11_565 .
O5A O5B Si1 75(10) 11_565 10_556
O5A O5B Si1 72(3) . 10_556
O5B O5B Si1 71.6(18) 11_565 10_556
Si1 O5B Si1 134(4) . 10_556
O5A O5B Rb4 119(10) 11_565 13
O5A O5B Rb4 129(8) . 13
O5B O5B Rb4 131.3(10) 11_565 13
Si1 O5B Rb4 112(2) . 13
Si1 O5B Rb4 112(2) 10_556 13
O5A O5B Rb3 154(10) 11_565 .
O5A O5B Rb3 143(8) . .
O5B O5B Rb3 141.3(11) 11_565 .
Si1 O5B Rb3 96.1(19) . .
Si1 O5B Rb3 96.1(19) 10_556 .
Rb4 O5B Rb3 87.5(14) 13 .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
U1 O1 1.841(8) .
U1 O1 1.841(8) 13
U1 O3 2.1373(14) .
U1 O3 2.1373(14) 13
U1 O2B 2.270(11) 13
U1 O2B 2.270(11) .
U1 O2A 2.291(11) .
U1 O2A 2.292(11) 13
U1 Rb2 3.8774(4) .
U1 Rb2 3.8774(4) 13
U1 Rb3 3.9920(2) 13
U1 Rb3 3.9920(2) .
Rb1 O1 2.944(9) 12
Rb1 O1 2.944(9) 11_565
Rb1 O1 2.944(9) 2_565
Rb1 O1 2.944(9) .
Rb1 O4 3.079(11) .
Rb1 O2B 3.206(11) .
Rb1 O2B 3.206(11) 11_565
Rb1 O2B 3.206(11) 12
Rb1 O2B 3.206(11) 2_565
Rb1 Si1 3.528(3) 2_565
Rb1 Si1 3.528(3) .
Rb1 O3 3.588(11) 2_565
Rb2 O2B 2.853(11) 14_445
Rb2 O2B 2.853(11) 8_455
Rb2 O2B 2.853(11) 13
Rb2 O2B 2.853(11) 7_545
Rb2 O3 3.111(10) .
Rb2 O3 3.111(10) 2
Rb2 O1 3.251(9) 13
Rb2 O1 3.251(9) 14_445
Rb2 O1 3.251(9) 7_545
Rb2 O1 3.251(9) 8_455
Rb2 O2A 3.374(11) 14_445
Rb2 O2A 3.374(11) 8_455
Rb3 O1 3.144(8) 8_455
Rb3 O1 3.144(8) 6
Rb3 O1 3.144(8) 15_455
Rb3 O1 3.144(8) 13
Rb3 O3 3.158(11) 10_556
Rb3 O3 3.158(11) .
Rb3 O5B 3.19(5) 3_556
Rb3 O5B 3.19(5) .
Rb3 O2A 3.253(11) 10_556
Rb3 O2A 3.253(11) 12
Rb3 O2A 3.253(11) 3_556
Rb3 O2A 3.253(11) .
Rb4 O2A 2.925(11) 15_454
Rb4 O2A 2.925(11) 13
Rb4 O2A 2.925(11) 8_455
Rb4 O2A 2.925(11) 6_554
Rb4 O5B 2.99(6) 15_454
Rb4 O5B 2.99(6) 13
Rb4 O5A 3.07(5) 5_444
Rb4 O5A 3.07(5) 7_545
Rb4 O1 3.172(9) 3
Rb4 O1 3.172(9) 10
Rb4 O1 3.172(9) 12
Rb4 O1 3.172(9) .
Si1 O2B 1.541(11) .
Si1 O2B 1.541(11) 11_565
Si1 O5A 1.610(19) .
Si1 O5A 1.610(18) 11_565
Si1 O2A 1.617(11) 11_565
Si1 O2A 1.617(11) .
Si1 O4 1.627(2) .
Si1 O5B 1.64(2) .
Si1 O5B 1.64(2) 11_565
Si1 Rb2 3.668(3) 13
O1 Rb3 3.144(8) 13
O1 Rb2 3.251(9) 13
O2A O2B 0.783(14) .
O2A Rb4 2.925(11) 13
O2A Rb2 3.374(11) 13
O2B Rb2 2.853(11) 13
O2B Rb4 3.572(11) 13
O3 U1 2.1373(14) 8_455
O4 Si1 1.627(2) 2_565
O4 Rb3 3.391(5) 9_566
O5A O5B 0.16(10) 11_565
O5A O5A 0.73(10) 11_565
O5A O5B 0.88(3) .
O5A Si1 1.610(18) 10_556
O5A Rb4 3.07(5) 5
O5A Rb3 3.33(5) 9_566
O5A Rb4 3.62(5) 13
O5B O5A 0.16(10) 11_565
O5B O5B 1.04(11) 11_565
O5B Si1 1.64(2) 10_556
O5B Rb4 2.99(6) 13
